Positional Flexibility: Syntheses and Characterization of Six Uranium Chalcogenides Related to the 2H Hexagonal Perovskite Family.
Mesbah, Adel; Prakash, Jai; Beard, Jessica C.; Pozzi, Eric A.; Tarasenko, Mariya S.; Lebègue, Sébastien; Malliakas, Christos D.; Van Duyne, Richard P.; Ibers, James A.; Inorganic chemistry 54 (2015) 2851–2857; doi:10.1021/ic5029806

data_4342469
_publ_section_title
;
 Positional Flexibility: Syntheses and Characterization of Six Uranium
 Chalcogenides Related to the 2H Hexagonal Perovskite Family.
;
_journal_issue                   6
_journal_name_full               'Inorganic chemistry'
_journal_page_first              2851
_journal_page_last               2857
_journal_paper_doi               10.1021/ic5029806
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'Ba3.3 Rb0.7 S6 U'
_chemical_formula_weight         943.05
_space_group_crystal_system      trigonal
_space_group_IT_number           167
_space_group_name_Hall           '-R 3 2"c'
_space_group_name_H-M_alt        'R -3 c :H'
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_audit_creation_method           SHELXL-2014/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   12.0875(3)
_cell_length_b                   12.0875(3)
_cell_length_c                   15.1516(5)
_cell_measurement_reflns_used    4701
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      59.865
_cell_measurement_theta_min      6.637
_cell_volume                     1917.18(9)
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.997
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0227
_diffrn_reflns_av_unetI/netI     0.0100
_diffrn_reflns_Laue_measured_fraction_full 0.995
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            7520
_diffrn_reflns_point_group_measured_fraction_full 0.995
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.055
_diffrn_reflns_theta_min         4.734
_exptl_absorpt_coefficient_mu    26.234
_exptl_absorpt_correction_T_max  0.60971
_exptl_absorpt_correction_T_min  0.39512
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'face indexed (SADABS; Sheldrick, 2008)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    4.901
_exptl_crystal_description       block
_exptl_crystal_F_000             2391.4
_exptl_crystal_size_max          0.068
_exptl_crystal_size_mid          0.041
_exptl_crystal_size_min          0.033
_refine_diff_density_max         0.519
_refine_diff_density_min         -0.653
_refine_diff_density_rms         0.112
_refine_ls_extinction_coef       0.000080(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.378
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         628
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.377
_refine_ls_R_factor_all          0.0104
_refine_ls_R_factor_gt           0.0094
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0065P)^2^] where P=(1.0000Fo^2^+0.0000Fc^2^)'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0193
_refine_ls_wR_factor_ref         0.0194
_reflns_Friedel_coverage         0.000
_reflns_number_gt                599
_reflns_number_total             628
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ic5029806_si_001.cif
_cod_data_source_block           Ba33Rb07US6
_cod_depositor_comments
'Adding full bibliography for 4342464--4342469.cif.'
_cod_original_cell_volume        1917.18(11)
_cod_database_code               4342469
_shelx_estimated_absorpt_t_min   0.266
_shelx_estimated_absorpt_t_max   0.476
_shelxl_version_number           2014/6
_shelx_res_checksum              12511
_shelx_hkl_checksum              86408